Polyurethane Nanofiber Membranes for Waste Water Treatment ... ResearchArticle Polyurethane...
Embed Size (px)
Transcript of Polyurethane Nanofiber Membranes for Waste Water Treatment ... ResearchArticle Polyurethane...
Research Article Polyurethane Nanofiber Membranes for Waste Water Treatment by Membrane Distillation
T. JilíIek,1 M. Komárek,2 and T. Lederer2
1Membrain s.r.o., Pod Vinićı 87, 47127 Stráž pod Ralskem, Czech Republic 2Technical University of Liberec, Studentská 1402/2, 46117 Liberec 1, Czech Republic
Correspondence should be addressed to T. Jiř́ıček; firstname.lastname@example.org
Received 23 February 2017; Accepted 11 April 2017; Published 7 May 2017
Academic Editor: Piotr Nowicki
Copyright © 2017 T. Jiř́ıček et al.This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Self-sustained electrospun polyurethane nanofiber membranes were manufactured and tested on a direct-contact membrane distillation unit in an effort to find the optimum membrane thickness to maximize flux rate and minimize heat losses across the membrane. Also salt retention and flux at high salinities up to 100 g kg−1 were evaluated. Even though the complex structure of nanofiber layers has extreme specific surface and porosity, membrane performance was surprisingly predictable; the highest flux was achieved with the thinnest membranes and the best energy efficiency was achieved with the thickest membranes. All membranes had salt retention above 99%. Nanotechnology offers the potential to find modern solutions for desalination of waste waters, by introducing newmaterials with revolutionary properties, but newmembranes must be developed according to the target application.
As the demands for potable water are rising every year and more stringent environmental legislation is issued, there is a clear need for the development of new technologies and materials to meet these challenges. Even though many new approaches are examined every day in order to find a solution with lower energy consumption, higher effectivity, and the possibility of using alternative energy sources, most novelties are not as durable and reliable as existing technologies, such as reverse osmosis (RO). Future prospects of RO, on the other hand, may seem quite complicated as the energy demands and brine production are both unsustainably high . In this perspective, membrane distillation (MD) is theoretically a very attractive alternative: not pressure but temperature driven up to saturated concentrates, with high salt rejection and possibility of being powered by solar or geothermal energy, or low-graded waste heat . What has always held MD from becoming a mainstream technology were suitable membranes, or more precisely the lack of them, which would provide fluxes comparable with traditional RO. Hence, the interest to develop new membranes specifically for MD has been quite intense in recent years .
When developing new membranes for MD, the max- imisation of membrane permeability and hydrophobicity in terms of bubble point pressure and contact angle are obviously desirable, as are low fouling and chemical and mechanical stability . Even though membrane thickness is a key parameter, its role is not quite straightforward, but at least it is generally acknowledged that thin membranes with large pores provide high fluxes and that thick membranes with small pores minimize heat losses via conduction . Even though approximate ranges were suggested, including a simulation using the Dusty Gas Model , there is still no clear understanding what the optimummembrane thickness is. Although nanotechnology has a significant potential role in membrane based desalination , information about optimum structural parameters for nonwoven membranes is even scarcer and therefore deeper study is most relevant. Nanofibers are typically created by an electrostatic field from a polymer solution by electrospinning  and both high porosity and hydrophobicity are declared [6, 7].
Electrospun nanofiber membranes have significantly bet- ter transmembrane fluxes than currently used hydrophobic microfiltration membranes [8, 9]. Polyfluorinated polymers that have been tested recently [10–12] displayed excellent
Hindawi Journal of Nanotechnology Volume 2017, Article ID 7143035, 7 pages https://doi.org/10.1155/2017/7143035
2 Journal of Nanotechnology
hydrophobicity, but they also prove electrospinning difficult, thus restraining the possibility for a deeper study involving many layers of varying properties. Polyurethane (PUR), on the other hand, allows for adjustment of membrane thickness both by varying substrate velocity and by placing several layers onto each other; moreover, they do not require any kind of mechanical support, thus avoiding a performance deteriorating step of thermal-pressure lamination .
The novelty of this work consists of electrospinning and testing nonlaminated, self-sustained PUR membranes for the application of MD in waste water treatment. Their performance was evaluated in terms of transmembrane flux, energy efficiency, and salt retention, including the test at various recirculation velocities and several different salt concentrations of the feed solution.
2. Materials and Methods
The flat sheet nanofiber PUR membranes were prepared by continuous needleless electrospinning process, using the NanoSpider� spinner (Elmarco). PUR resin (Lar- ithane Al286, Novotex Italiana S.p.A., molecular weight 2000 gmol−1, technical grade quality, supplied as 30% w./w. solution in DMF) and N,N-dimethylformamide (Sigma- Aldrich) were both used as received. The polymer solution was prepared by dissolving the PUR polymer in DMF. The polymer concentration was set to 18% w./w. The solution was stirred for 2 hours at 21∘C on a magnetic stirrer in a sealed beaker to prevent the solvent evaporation.
NanoSpider� is equipped with a 0.2mm wire emitting electrode and a static wire collecting electrode. The polymer solution is applied on the emitting electrode by a moving applicator. Both electrodes are attached to the high voltage power supply.The voltage between electrodeswas set to 70 kV and the distance between the electrodes was kept constant at 175mm. Relative humidity in the electrospinning chamber was kept below 20% at 24∘C to minimize the formation of defects. The nanofibers were collected on a nonadhesive paper substrate passing between emitting and collecting electrode. Production speed varied according to the desired nanofiber membrane sheet thickness.
Four different individual membranes were manufactured with a varying surface density in grams per square meter (GSM) to be 6, 10, 25, and 40 gm−2, designated as PUR06, PUR10, PUR25, and PUR40. The lower weight membranes (6 and 10 gm−2) were prepared in one step by variation of the substrate speed. The two thicker membranes were prepared by multiple passing of the substrate material through the spinning chamber, PUR25 by 3 passes and PUR40 by 5 passes. The prepared nanofiber membranes were designed to be self-supporting; thus lamination process was not necessary. Mechanical properties of the PURmembranes were sufficient for handling of the membranes and application in MD.
The membranes were tested on a laboratory scale direct- contact (DCMD) unit with a 0.02m2 flat sheet module. Countercurrent recirculation was powered by a peristaltic pump with two rotors. Two feed temperatures of 50 and 60∘C were tested, in order to assess the potential thermal dete- rioration of not-so-temperature-resistant PUR membranes.
Temperatures were measured via four thermocouples in the module inlet and outlet pipes. Two hot baths, Julabo F12 and Lauda RE 420, were used to set the driving force according to the logarithmic mean temperature difference (LMTD) and were kept at 10∘C in all the experiments.
(i) Transmembrane flux was evaluated with deminer- alized water in both feed and distillate circuits, with cross-flow velocity ranging between 60 and 90mm s−1, and was calculated as a difference in the distillate mass on a A&D EK-12Ki scale.
(ii) Membrane retention was tested with various sodium chloride concentrations in the feed solution, up to approximately 100 g kg−1, and it was calculated as
𝑅 = 1 − 𝑐𝑑 𝑐𝑓 , (1)
where 𝑐𝑓 is the feed concentration and 𝑐𝑑 is the distillate concentration. The electrical conductivity was measured by WTW TetraCon probes connected to WTWMutli9430 and WTWMulti350i.
(iii) Flux decline with increasing feed concentration was measured at approximately 85mm s−1.
(iv) Energy efficiency was measured at four circulation velocities (60, 70, 80, and 90mm s−1) and calculated as
𝐸 = 𝑁 ⋅ 𝑑𝐻 ⋅ 𝐴
𝑚 ⋅ 𝐶𝑝 ⋅ 𝑑𝑇 , (2)
where 𝑁 is flux, dH is the enthalpy of condensation, 𝐴 is the membrane area,𝑚 is the mass flow rate along the membrane, Cp is the heat capacity, and dT is the temperature difference at the inlet and outlet of the module.
POROMETER 3G (Quantachrome) was used to measure the bubble point pressure and pore sizes by a wet-dry flow method. Optical Tensiometer THETA QC (Attension) was used to measure the contact angle with demineralized water, giving an average of the right and left angle.
Tescan Vega3SB (CZ) was used to study the membrane structure and thickness. This high vacuum scanning elec- tron microscope measures the Au/Pt coated samples at an acceleration voltage of 30.0 kV. The cross section thicknesses of the membranes were obtained by breaking the frozen membranes in liquid nitrogen. To obtain the fiber dimensions and membrane thickness, image analysis was done in Tescan software.
3. Results and Discu